Received: 7 April 2017 Accepted: 3 July 2017 Published online: 4 August 2017
Size effect on atomic structure in low-dimensional Cu-Zr amorphous systems W. B. Zhang1, J. Liu1, S. H. Lu2, H. Zhang3, H. Wang4, X. D. Wang1, Q. P. Cao1, D. X. Zhang5 & J. Z. Jiang1 The size effect on atomic structure of a Cu64Zr36 amorphous system, including zero-dimensional smallsize amorphous particles (SSAPs) and two-dimensional small-size amorphous films (SSAFs) together with bulk sample was investigated by molecular dynamics simulations. We revealed that sample size strongly affects local atomic structure in both Cu64Zr36 SSAPs and SSAFs, which are composed of core and shell (surface) components. Compared with core component, the shell component of SSAPs has lower average coordination number and average bond length, higher degree of ordering, and lower packing density due to the segregation of Cu atoms on the shell of Cu64Zr36 SSAPs. These atomic structure differences in SSAPs with various sizes result in different glass transition temperatures, in which the glass transition temperature for the shell component is found to be 577 K, which is much lower than 910 K for the core component. We further extended the size effect on the structure and glasses transition temperature to Cu64Zr36 SSAFs, and revealed that the Tg decreases when SSAFs becomes thinner due to the following factors: different dynamic motion (mean square displacement), different density of core and surface and Cu segregation on the surface of SSAFs. The obtained results here are different from the results for the size effect on atomic structure of nanometer-sized crystalline metallic alloys. The atomic structure of metallic glasses (MGs) is a long-standing unsolved issue in condensed matter community1–3. Considerable efforts have been made to describe the structure and/or to reveal various factors influencing atomic structure of metallic glasses by experiments4, 5 and simulations6, 7, such as cooling rate8–10 and composition11–13. The sample size effect on properties of MGs has been reported, e.g., size effect on stability14, strength15–18, ductility19–21, elastic limit22–24, plasticity and deformation mode25–30. However, the size effect on atomic structure of low-dimensional amorphous systems, including zero-dimensional small-size amorphous particles (SSAPs) and two-dimensional small-size amorphous thin films (SSAFs) has not been systematically reported yet, possibly because the precise fabrication of free standing SSAPs and SSAFs with various sizes, while keeping the thermal history invariant, is rather difficult if not impossible. In crystalline metallic particles, the smaller the particles, the stronger the sample size effect on atomic structure. Atomistic simulations have been widely applied to study the structure of nanometer-sized crystalline metallic particles31–35 and thin films36, 37. Thus, we resort to atomistic simulations to study the size-dependent atomic structure in SSAPs and SSAFs. In this work, we report the results of atomic structures in a zero-dimensional Cu64Zr36 SSAPs, ranging from about 11 Å to 60 Å in diameter, and in a two-dimensional Cu64Zr36 SSAFs, ranging from 8.6 Å to 61.5 Å in thickness as a prototype model system in which the Cu-Zr potential was well developed and applied27–30, 38–41, by molecular dynamics simulations. It is found that sample size strongly affects local atomic structure in Cu64Zr36 SSAPs and SSAFs, which are composed of core and shell components in SSAPs and of core and surface layers in SSAFs. Each component has different atomic packing structure, average coordination number, bond length, and the degree of ordering. These atomic 1
International Center for New-Structured Materials (ICNSM), Laboratory of New-Structured Materials, State Key Laboratory of Silicon Materials, and School of Materials Science and Engineering, Zhejiang University, Hangzhou, 310027, People’s Republic of China. 2School of Materials Science and Engineering, Zhejiang University of Technology, Hangzhou, 310014, People’s Republic of China. 3Department of Chemical and Materials Engineering, University of Alberta, Edmonton, Alberta, T6G 2V4, Canada. 4Institute of Nanosurface Science and Engineering, Shenzhen University, Shenzhen, 518060, People’s Republic of China. 5State Key Laboratory of Modern Optical Instrumentation, Zhejiang University, Hangzhou, 310027, People’s Republic of China. W.B. Zhang and J. Liu contributed equally to this work. Correspondence and requests for materials should be addressed to J.Z.J. (email: [email protected]
) SCIENTIfIC REPOrtS | 7: 7291 | DOI:10.1038/s41598-017-07708-5
Figure 1. Pair distribution functions g(r) for Cu64Zr36 SSAPs with various sizes together with bulk sample for the (a) total, (b) core component together with an illustration of the core-and-shell model in the inset and (c) shell component.
structure differences in Cu64Zr36 SSAPs and SSAFs with various sizes or thicknesses result in different glass transition temperatures, in which the glass transition temperature for the shell component is found to be 577 K, which is much lower than 910 K for the core component in SSAPs while Tg decreases with the thickness of SSAFs. It has been manifested unambiguously that free surface is the dominant cause for Tg reductions. Cu atoms segregate to the surface causing a far higher concentration while the core component almost remains the same composition as films. The finding obtained here will trigger more studies on the unsolved puzzle of atomic structure in disordered materials in general.
Results and Discussion
Pair distribution functions in Cu64Zr36 SSAPs. For Cu64Zr36 SSAPs with various sizes together with bulk
sample at T = 300 K were plotted in Fig. 1a while partial pair distribution functions for Cu64Zr36 SSAPs with various sizes are plotted in Fig. 2. The g(r) of Cu64Zr36 SSAPs even for a size of 50 atoms still exhibit a relative sharp first peak and a split second peak, which were characteristic of amorphous. The intensity of the first peak increases with the size, while the g(r) for larger sized Cu64Zr36 SSAPs (4000 and 5000 atoms) becomes similar to that of bulk Cu64Zr36 MG. In the range of 4–6 Å, i.e., for the second and third neighbors, g(r) are different from 50 atoms to 700 atoms, while after 700 atoms, they are similar to the bulk sample. The partial pair distribution functions g(r) of Cu-Cu, Cu-Zr, and Zr-Zr pairs in Fig. 2 show the increase in intensity of the first peak with sample size while the positions of the peaks in partial g(r) remain almost unchanged, indicating the average atomic bonds are not sensitive to particle size. The first peak distance becomes larger as particle size increases. A similar observation is also found in nanometer-sized crystalline ZnS particles42, 43. To dig out details of local atomic structure in particles, the core-and-shell model in the inset of Fig. 1b is applied, in which the thickness SCIENTIfIC REPOrtS | 7: 7291 | DOI:10.1038/s41598-017-07708-5
Figure 2. Pair distribution functions g(r) for Cu64Zr36 SSAPs with various sizes together with bulk sample for the (a) total, (b) Cu-Cu partial, (c) Cu-Zr partial, (d) Zr-Zr partial. Number of atoms Components Parameters Total core shell
Position (Å) (±0.01)
Position (Å) (±0.01)
Position (Å) (±0.01)
Table 1. The position and average coordination number of the first peak in g(r) for Cu64Zr36 SSAPs total sample, and core and shell components.
of shell was estimated by the minimum after the first peak in total g(r) to be about 3.7 Å. In general, it is tough to select the shell layer thickness for nanometer-sized particles, which depends on materials and properties one selected. From the atomic packing short-range order point of view, using the first minimum in the g(r) here is not an unreasonable value14. It should be mentioned that normally the thickness of the shell could also be a function of particle size. However, the minimum position after the first peak in total g(r) in Fig. 1a is roughly unchanged by varying particle sizes. Corresponding pair distribution functions g(r) for the core and shell components are plotted in Fig. 1b and c, respectively. For the 50-atom particle, almost all atoms are located in the shell component, reflected by the similar g(r) for both total and shell. By increasing particle size, the fraction of atoms in the core component increases. From 50 to 700 atoms, the g(r) in the range of 4–6 Å largely change in both core and shell components. Above 700 atoms, g(r) for the core component are similar to the total g(r), while g(r) for the shell component does not change much for 1000, 4000 and 5000 atoms. It is found that the first peak positions in g(r) for the core component are larger than those for the shell component in Table 1, revealing larger average bond lengths in the core component than those in the shell component, which might be linked with different coordination numbers and/or compositions in shell and core components, discussed later. It shows that the total average bond length has a tend to decrease with the size decreasing of nanoparticles from 2.78 Å to 2.73 Å, which means that the nanoparticle shrunk. It can be concluded from pair distribution functions that atomic structures in both core and shell components largely differ in Cu64Zr36 SSAPs with sizes from 50 to 700 atoms while atomic structures in particles with sizes above 1000 atoms are similar.
Coordination number distributions and short range atomic packing in Cu64Zr36 SSAPs. The coordination number (CN) distribution of the total particle, and core and shell components in Cu64Zr36 SSAPs are SCIENTIfIC REPOrtS | 7: 7291 | DOI:10.1038/s41598-017-07708-5
Figure 3. The coordination number distributions of the total sample, core and shell components, (a–c) for both elements, (d–f) for only Cu-centered atoms, and (g–i) for only Zr-centered atoms, respectively. The inset in (f) is the 5000-atom particle with red balls as Cu atoms and blue balls as Zr atoms.
further calculated in Fig. 3. The CN distribution in total particles show a bi-peak distribution centered at about CN = 7 and 12, which strongly depends on the size of SSAPs. With increasing the particle size, the fraction of atoms with high CN increase at the expense of the fraction of atoms with low CN. The bi-peak distributions are clearly linked with the CN distributions of the core and shell components in Fig. 3b and c, respectively. In the core component, CN distributes in the range of CN = 10–16 while in the shell component, it distributes from CN = 5 to CN = 10. This lower CN in the shell component can be explained by the surface effect while higher CN in the core component reveals relative dense atomic packing in Cu64Zr36 SSAPs. Similar to g(r), it is found that CN distribution in both core and shell components strongly depend on the particle size in the range 50–700 atoms while it remains almost steady for particle size larger than 700 atoms. In terms of Cu- and Zr-centered surroundings in total particles, core and shell components in Fig. 4d–i, the CN of Cu atoms in the core component is centered at about 12 and about 14 for Zr atoms. However, the CN of Zr atoms in the shell component still have higher CN (>9) compared with Cu atoms (CN